## Application a direct/cohesive zone

## method for the evaluation of scarf adhesive

## joints

### D. F. O. Silva

1_{, R. D. S. G. Campilho}

1,2*_{ , F. J. G. Silva}

1_{ and U. T. F. Carvalho}

1
**Introduction**

The use of adhesive bonds in the aerospace, aeronautical and automotive industries,
among others, has assumed a high preponderance to the detriment of conventional
joining methods such as riveting, bolting, brazing and welding. In fact, adhesive bonds
offer several advantages such as the reduction of stress concentrations, good response
to fatigue stresses, ability to bond dissimilar materials and lightness of structures.
How-ever, they also present some limitations, namely the difficulty of disassembly, high cure
times (in some cases) and limited temperature and humidity conditions [1]. The strength
and behaviour of adhesive bonds depends on several factors, namely the type of
adhe-sive used, the material of the adherends, the joint configuration and dimensional factors,
such as the overlap length (*L*O) and the adhesive and adherends’ thickness (*t*A and *t*P,

respectively). There are several types of joint geometries, although the most common are single-lap, double-lap and scarf [2–5]. Scarf joints are modified butt joints that are

**Abstract**

With the increasing use of structures with adhesive bonds at the industrial level, several
authors in the last decades have been conducting studies concerning the behaviour
and strength of adhesive joints. Between the available strength prediction methods,
cohesive zone models, which have shown good results, are particularly relevant. This
work consists of a validation of cohesive laws in traction and shear, estimated by the
application of the direct method, in the strength prediction of joints under a
mixed-mode loading. In this context, scarf joints with different scarf angles (*α*) and adhesives
of different ductility were tested. Pure-mode cohesive laws served as the basis for the
creation of simplified triangular, trapezoidal and exponential laws for all adhesives.
Their validation was accomplished by comparing the numerical maximum load (*P*_{m})
predictions with the experimental results. An analysis of peel (*σ*) and shear (*τ*) stresses
in the adhesive layer was also performed to understand the influence of stresses on

*P*_{m}. The use of the direct method allowed obtaining very precise *P*_{m} predictions. For
the geometric and material conditions considered, this study has led to the conclusion
that no significant *P*_{m} errors are incurred by the choice of a less appropriate law or by
uncoupling the loading modes.

**Keywords:** Adhesive joint, Structural adhesive, Finite elements, Cohesive zone model,
Scarf joint

**Open Access**

© The Author(s) 2018. This article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creat iveco mmons .org/licen ses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.

**RESEARCH**

more time-consuming to fabricate (i.e., they require milling operations). This type of
joint, when loaded, has the ability to keep the axis of loading aligned with the joint [6].
Besides that, it allows a practically constant stress distribution when manufactured with
an optimized value of *α*. Because of this, scarf joints are popular to join composite parts
[7]. However, this joint type fails to work under bending, because this loading induces
cleavage stresses in the adhesive [1].

Over the years, reliable and accurate strength prediction techniques were developed.
Two distinct approaches can be followed: analytical and numerical. The analytical
tech-niques are able to easily obtain the stress state in bonded structures due to assuming
simplifying assumptions in terms of joint geometry, loading and boundary conditions,
allowing to obtain an explicit analytical solution for the behaviour in the elastic domain
[8, 9]. Nowadays, numerical methods are often preferred over analytical ones, since they
overcome some limitations of the analytical methods, such as the possibility to include
some effects such as non-linearity of the adhesive and adherends, or to consider
geo-metrical non-linearities [10]. The most common numerical method applied to adhesive
bonds is CZM, as a modification of the conventional continuum-based finite element
method (FEM) formulation [11, 12]. The extended finite element method (XFEM) is a
more recent technique that has showed promising results in the simulation of bonded
joints [13, 14]. CZM has been extensively used in the simulation of the structures’
behav-iour until failure, since it allows to include in the numerical models the possibility of
multiple failure paths in different regions of the materials or between interfaces, which is
very helpful for adhesive joints [15]. CZM laws are based on a relationship between the
cohesive stresses in tension (*t*n) and shear (*t*s) with the relative displacements in tension

(*δ*n) and shear (*δ*s) that link homologous nodes of the cohesive elements [16]. The work

of Rocha and Campilho [17] analysed the effect of using different CZM conditions in modelling single-lap joints under a tensile loading. The following analyses were made: variation of the CZM laws’ elastic stiffness, different mesh refinements in the crack paths, study of the adherends’ element type, and evaluation of several damage initiation and growth criteria. It was shown that CZM is suitable for static strength prediction of bonded joints, and the best set of numerical conditions for this purpose was pointed out.

The main parameters of the CZM laws to introduce in the numerical models are
the cohesive strengths in tension (*t*n0) and shear (*t*s0), and the critical values of tensile

and shear strain energy release rate (*G*IC and *G*IIC, respectively). The estimation of the

referred cohesive parameters (*G*IC, *G*IIC, *t*n0 and *t*s0) can be performed by the property

identification technique, the inverse method and the direct method. All these methods
usually rely on double-Cantilever Beam (DCB) or End-Notched Flexure (ENF) tests. The
property identification technique consists of the isolated definition of the cohesive laws
parameters through appropriate tests, while the inverse method relies on estimating at
least one parameter by an iterative adjustment procedure between experimental data of
a given test and its FEM prediction [18]. In a typical inverse method approach, *G*IC and

*G*IIC are estimated by tests such as the DCB and ENF, respectively, using a suited method

or theory. Then, the obtained values of *G*IC and *G*IIC are used to build CZM laws in pure

modes (tension and shear), while typical values of the parameters *t*n0 and *t*s0 are initially

both divided by *t*A. These CZM laws are next applied to numerical models replicating

the fracture tests, created with the same dimensions of the real specimens. Following,
for the definition of *t*n0 and *t*s0, an adjustment is undertaken between the numerical and

experimental load–displacement (*P*–*δ*) curves, producing a cohesive law that can
accu-rately reproduce the adhesive layer in the respective loading mode. The assembly of a
mixed-mode CZM from this information, including criteria for damage initiation and
growth prediction, enables to design bonded structures under arbitrary loadings. This
method was applied in the work of Moreira and Campilho [6], to assess the strength
improvement of bonded scarf repairs in aluminium structures with distinct external
reinforcements, using the adhesive Araldite® 2015 (Araldite® from Huntsman, Basel,
Switzerland). Fairly accurate numerical approximations were attained, but generally
with slightly smaller *P*m values compared to the experiments. The maximum deviation

attained was 20.2%, for a specific repair configuration. This allowed to conclude that
the used numerical technique and respective inverse method for CZM laws
establish-ment simulate with reasonable accuracy the behaviour of the bonded repairs. The direct
method allows estimating the complete cohesive law for a given material or interface by
differentiating the tensile strain energy release rate (*G*I) or the shear strain energy release

rate (*G*II) with respect to *δ*n or *δ*s, after the polynomial fitting to the most precise degree.

With this procedure, the tensile and shear cohesive laws can be obtained, for example,
from DCB and ENF tests, respectively [19]. The accuracy of the obtained cohesive laws
can be verified by comparing the *P*–*δ* curves resulting from CZM laws simulation with
the respective test results. A few works are available that estimate the CZM laws of
adhe-sives by the direct approach from either pure or mixed-mode fracture tests. For instance,
in the work of Ji et al. [20], the DCB specimen was used to estimate the CZM laws in
tension of a brittle epoxy adhesive by a direct method. A clear tendency was achieved as
a function of *t*A: (1) *G*IC increases up to *t*A= 1 mm and (2) *t*n0 is highest for *t*A= 0.09 mm

and slowly reduces by increasing *t*A up to equalling the bulk strength of the adhesive.

Leffler et al. [21] used the ENF specimen to calculate *G*IIC and the CZM law in shear

of an epoxy adhesive by the direct method. Constant displacement rate and constant
shear deformation rate assumptions were compared, giving identical estimations of *t*s0.

On the other hand, higher *G*IIC was found by testing at constant displacement rate. Jumel

et al. [22] directly addressed the mixed-mode CZM laws of adhesive layers by using the
mixed-mode bending (MMB) test. Gheibi et al. [23] proposed a new mode-dependent
CZM for the simulation of adhesive joints, estimated by the direct method. This was
accomplished by using DCB and ENF tests for the direct experimental extraction of the
CZM laws (tensile and shear, respectively). The obtained laws were used to implement a
simplified Park–Paulino–Roesler CZM. After deriving the mixed-mode parameters, the
proposed model was implemented in Abaqus® (Dassault Systèmes, Vélizy-Villacoublay,
France) and validated against experimental results of single-lap joints and scarf joints.
The accuracy of the developed mixed-mode CZM model for was confirmed for different
mode-mixity conditions. The direct method was also applied in the work of Carvalho
and Campilho [24] to validate, with a mixed-mode geometry, tensile and shear
cohe-sive laws obtained in pure mode. With this purpose, single lap-joints with different *L*O

triangular, trapezoidal and linear–exponential CZM laws in order to evaluate which
form fits better with the behaviour of each adhesive. The joints bonded with the brittle
Araldite® AV138 were best modelled by a triangular CZM law shape, mainly due to the
adhesive’s brittleness, while the Araldite®_{ 2015 results were best fitted with a }

trapezoi-dal CZM, considering that this adhesive has some degree of ductility. The behaviour of the highly ductile Sikaforce® 7752 (Sikaforce® from Sika®, Baar, Switzerland) was more accurately reproduced by a trapezoidal CZM law. However, irrespectively of the adhe-sive, for the analysed joint geometry (single-lap joints), the errors incurred by applying a less suitable CZM law shape for a given adhesive were always under 10%.

This work consists of a validation of cohesive laws in traction and shear, estimated by
the application of the direct method, in the strength prediction of joints under a
mixed-mode loading. In this context, scarf joints with different *α* values and adhesives of
differ-ent ductility were tested. Pure-mode cohesive laws served as the basis for the creation of
simplified triangular, trapezoidal and exponential laws that were tested for each of the
adhesives. Their validation was accomplished by comparing the numerical *P*m

predic-tions with the experimental results. An analysis of *σ* and *τ* stresses was also performed in
the adhesive layer in order to understand the influence of stresses on the joints’ strength.

**Methods**
**Experimental**

**Adherends and adhesives**

The adherends used in the DCB, ENF and scarf specimens consisted of the
AW6082-T651 aluminium alloy. This material is obtained through artificial aging, at a
tempera-ture of 180 °C, and it was selected due not only to its attractive mechanical properties,
but also to the wide field of structural applications in extruded and laminated
prod-ucts. It was characterized in previous studies [25], where the following properties were
defined: tensile strength of 324.00 ± 0.16 MPa, *E* of 70.07 ± 0.83 GPa, yield stress of

261.67 ± 7.65 MPa and tensile failure strain of 21.70 ± 4.24%. The stress–strain (*σ*–*ε*)
curves of this alloy were experimentally obtained according to the standard
ASTM-E8M-04 [25]. The adhesives selected for this work cover a range of ductility from low
(brittle) to high. The adhesives were the Araldite®_{ AV138, which is a brittle epoxy }

adhe-sive, the Araldite® 2015, an epoxy adhesive with moderate ductility, and the Sikaforce®
7752, a highly ductile polyurethane adhesive. Details regarding these adhesives can be
found in previous studies [26–28]. The DCB test was used to extract *G*IC and the ENF

test for *G*IIC. The collected data of the adhesives is given in Table 1.

**Joint geometry, fabrication and testing**

The geometry of the DCB (a) and ENF specimens (b) is shown in Fig. 1. These
speci-mens have the following dispeci-mensions: length *L*= 143 mm for the DCB and mid-span

*L*= 100 mm for the ENF, initial crack length *a*0≈ 55 mm, *t*P= 3 mm, *t*A= 0.2 mm and

width *B*= 25 mm. The scarf joints’ geometry is depicted in Fig. 2. The scarf joint has
a length (*L*T) of 200 mm, whilst the other dimensions are as follows: *B*= 25 mm,

*t*A= 0.2 mm, *t*P= 3 mm and *α* of 3.43°, 10°, 15°, 20°, 30° and 45°. The DCB and ENF joint

in order to remove oxide layers, and increase surface roughness, contact area and
wet-tability, to further improve the bonding process. After this procedure, all the adherends
were subjected to a chemical passive solvent degreasing process (cleaning with acetone)
in order to remove grease spots or abrasive particles [29]. With this procedure,
cohe-sive failures of the adhecohe-sive were achieved for all specimens. For the bonding process,
**Table 1 Properties of the adhesives Araldite**®** _{ AV138, Araldite}**®

**®**

_{ 2015 and Sikaforce}

_{ 7752 }**[26–28]**

a_{ Manufacturer’s data}

b_{ Estimated in Campilho et al. [}_{25}_{]}

**Property** **AV138** **2015** **7752**

Young’s modulus, E (GPa) 4.89 ± 0.81 1.85 ± 0.21 0.49 ± 0.09

Poisson’s ratio, ν 0.35a _{0.33}a _{0.30}a

Tensile yield stress, σ_{y} (MPa) 36.49 ± 2.47 12.63 ± 0.61 3.24 ± 0.48

Tensile failure strength, σf (MPa) 39.45 ± 3.18 21.63 ± 1.61 11.48 ± 0.25

Tensile failure strain, εf (%) 1.21 ± 0.10 4.77 ± 0.15 19.18 ± 1.40

Shear modulus, G (GPa) 1.56 ± 0.01 0.56 ± 0.21 0.19 ± 0.01

Shear yield stress, τy (MPa) 25.1 ± 0.33 14.6 ± 1.3 5.16 ± 1.14

Shear failure strength, τf (MPa) 30.2 ± 0.40 17.9 ± 1.8 10.17 ± 0.64

Shear failure strain, γf (%) 7.8 ± 0.7 43.9 ± 3.4 54.82 ± 6.38

*G*_{IC} (N/mm) 0.20b _{0.43 }_{±}_{ 0.02} _{2.36 }_{±}_{ 0.17}

*G*_{IIC} (N/mm) 0.38b _{4.70 }_{±}_{ 0.34} _{5.41 }_{±}_{ 0.47}

**Fig. 1** DCB (**a**) and ENF (**b**) test specimens for tensile and shear characterization of the adhesive layer,
respectively

spacers were used to ensure a constant value of *t*A and also to promote the creation of

the crack. In the DCB and ENF specimens, two calibrated spacers for each specimen
were used: a rear one, which allows to ensure a constant *t*A of 0.2 mm, and a front one

that, besides contributing to the constant *t*A, also enables creating a pre-crack. The

cur-ing of the adhesives was carried out in a prepared jig to ensure the adherends’
align-ment, taking into account the manufacturer specifications. After complete cure of the
adhesives, the adhesive excesses of all the samples were removed with the aid of a drill
press equipped with a grinding wheel. For the scarf joints, the fabrication began by
cut-ting the adherends from aluminium strips with dimensions of 140 mm (length), 25 mm
(width) and 3 mm (thickness). After this process, one of the adherends’ ends was milled
in a milling machine to obtain the respective *α*. Following, the scarf surfaces were
pre-pared for bonding identically to the DCB and ENF specimens. Bonding and curing were
undertaken using a jig that guaranteed the correct spacing between adherends, to
pro-mote the desired *t*A.

All joints were tested in the Shimadzu AG–X test equipment (Shimadzu, Kyoto,
Japan), with a 100 kN load cell. For the DCB and scarf tests, the machine was in the
generic configuration to perform tensile tests. For the ENF tests, it was adapted to apply
a three-point bending flexure loading. The equipment is connected to a data acquisition
system that records the test time, applied load and grips’ displacement. These values will
be used to plot the *P*–*δ* curves and perform all required data analysis. All the tests were
carried out under conditions of room temperature and humidity. The test velocity was
1 mm/min. Five specimens were tested for each condition.

**Direct method for the DCB and ENF tests**

The *J*-integral is suitable for the non-linear elastic behaviour of the materials, but
remains applicable for monotonic plastic loads. Based on the fundamental expression
for *J* defined by Rice [30], it is possible to derive an expression for *G*I applied to the DCB

specimen, from the concept of energy force and also by the beam theory for this particu-lar geometry, as follows

where *P*u represents the load per unit width applied at the specimen ends, *a* is the crack

length, *E*x is the Young’s modulus of the adherends, *θ*o is the relative rotation of the

adherends at the crack tip, and *θ*p is the relative rotation of the adherends measured at

the loading line. Figure 3 describes the direct method application to the tensile (a) and
shear (b) cohesive law estimation, with emphasis to the parameters *δ*n, *θ*o and *θ*p (DCB

test) and *δ*s (ENF test), necessary by the direct method, the relative displacement at *t*n0

(expressed as *δ*n0) and at *t*s0 (expressed as *δ*s0), and the tensile and shear relative

displace-ments at failure (*δ*nf and *δ*sf, respectively). The *t*n(*δ*n) curve can easily be obtained by

differ-entiating Eq. (1) with respect to *δ*n. In the work of Constante et al. [31], an experimental

work was carried out with the objective of estimating *G*IC of adhesive joints by the DCB

test. An optical measurement method was developed to evaluate *δ*n and *θ*o, to apply the

*J*-integral. It is also possible to apply a similar *J*-integral technique for *G*IIC estimation

(1)

G_{I}=12(Pua)

2

E_{x}t3

P

using the ENF test. The proposed *G*II evaluation expression results from the use of

alter-native integration paths to extract the *J*-integral, defined by Rice [30], resulting in the
following closed-form expression for the calculation of *G*II

The *t*s(*δ*s) curve or shear cohesive law of the adhesive layer is thus estimated by fitting

the resulting *G*II–*δ*s curve, and differentiation with respect to *δ*s. Leitão et al. [32]

pre-sents the full details regarding the description of the direct method applied to the ENF
specimen, as well as the algorithm to estimate *δ*s.

**Numerical**

**CZM theory**

In this work, approximated triangular, trapezoidal and linear–exponential laws were
tested to reproduce the experimentally obtained CZM laws by the direct method and
further undergo the validation process by comparing with experiments. In these three
models (further addressed as independent-mode models), the tensile and shear
behav-iours are uncoupled. The three CZM shapes are depicted in Fig. 4. In this figure, *δ*ns and

*δ*ss are the tensile and shear stress softening onset displacements of the trapezoidal CZM

law, respectively. The values *δ*nf and *δ*sf are internally calculated by the software from the

knowledge that the area under the CZM laws is equal to *G*IC (tensile law) or *G*IIC (shear

law). A mixed-mode triangular CZM model is also considered for comparison. In all

(2)

G_{II}= 9

16

(P_{u}a)2

E_{x}t3

P

+3

8

P_{u}δs

t_{P} .

models, the initial part of the CZM laws is defined by the relation between the current stresses and strains in tension and shear (subscripts n and s, respectively) [33]

The strain vector includes the tensile (*ε*n) and shear strain (*ε*s). The approximation of

making *K*nn=*E*, *K*ss=*G*, *K*ns= 0 is commonly accepted for the simulation of thin

adhe-sive layers [25]. In the independent-mode models, after *t*n0 and *t*s0, the softening portions

of the CZM law are based on the establishment of a damage variable (*d*n for tension or *d*s

for shear), such that [33]

where *t*nund and *t*sund are the current values of *t*n and *t*s, respectively, without stiffness loss

from the initial behaviour. The damage variable ranges between *d*n,s= 0 (in the elastic

portion of the CZM law) and *d*n,s= 1 (at the end of the softening process). More details

on the definition of this variable are available in Ref. [27]. The definition of *d*n,s for all

CZM law shapes is available in the Abaqus®_{ documentation [}_{33}_{]. The formulae for }

the linear–exponential law requires defining the parameter *α*exp to specify the

soften-ing evolution with *δ*n,s (*α*= 0 gives a triangular law and increasing *α*exp progressively

decreases stresses in the softening part of the curve). A value of *α*exp= 7 was

consid-ered in this work. Also, as previously mentioned, no coupling criteria was applied, i.e., the tensile and shear modes are independent in the simulations during damage growth, since this is the available method available in Abaqus®, which can be readily applied by users with less experience and knowledge. Naturally, the employed simplification can only be applied if the predictive capabilities of the method are not compromised. This was checked in a previous work [24], in which uncoupled-modes results are compared with those using a mixed mode triangular CZM, with positive results. In the triangu-lar mixed-mode model, a quadratic stress criterion was considered for damage initiation and a linear energetic criterion was used for damage growth. More details about this model can be found in Ref. [25].

(3)

**t**=

t_{n}
t_{s}

=

K_{nn} K_{ns}
K_{ns} K_{ss}

.

εn

εs

=**K**ε.

(4)

t_{n}=(1−d_{n}_{)}tund

n

t_{s}=(1−d_{s}_{)}tund

s ,

* Implementation of the model in Abaqus*®

The pure mode CZM laws in tension (*t*n–*δ*n) and shear (*t*s–*δ*s), obtained by the direct

method, were validated in Abaqus®, considering two-dimensional (2D) FEM models of
the scarf joints and a geometrically non-linear failure analysis [34]. Two distinct
mod-els were built: one for the elastic stress analysis and the other for the damage variable
(SDEG) analysis and for the CZM strength predictions. Considering the bondline stress
analysis, continuum FEM elements were applied in the adhesive layer and adherends,
while for the strength predictions the adhesive layer was modelled by one layer of CZM
elements in the thickness direction. The created models for stress analysis purposes
were meshed throughout by 4-node plane-strain elements (CPE4 from Abaqus®_{). For }

the strength analysis, the adherends were modelled as continuum elasto-plastic parts
with CPE4 elements, while the adhesive layer’s behaviour was characterized by a single
row of CZM elements, used to connect both adherends (COH2D4 4-node cohesive
ele-ments from Abaqus®) [27]. Figure 5 represents the mesh details for a scarf joint example
with *α*= 45° used for strength prediction. For both analysis types, the adhesive layer was

meshed with CZM elements’ with size of 0.1 mm (length) × 0.2 mm (thickness).
Assum-ing this procedure, the total number of CZM elements increases with the *α* reduction. In
order to minimize the computational effort, a mesh growth refinement was applied (bias
ratio) [35] in the adherends’ length direction, from the specimen’s ends to the beginning
of the scarf region. To simulate the real conditions of the experimental tests, as
bound-ary conditions, the joints were clamped at one end, and pulled in tension on the opposite
end, while orthogonally restrained.

**Results and discussion**

**CZM law estimation by the direct method**

In order to obtain the CZM laws for each one of the adhesives with the direct method,
first of all, it is necessary to estimate the *G*I–*δ*n and *G*II–*δ*s curves as mentioned in “0”

section, respectively, with Eqs. (1) and (2). A differentiation procedure is applied to
the referred curves after the polynomial fitting, to provide the complete CZM laws
in each pure mode. Figure 6 represents CZM curves’ examples for each adhesive
obtained from the DCB and ENF tests, all of them with the respective polynomial
fitting law, considering the adhesives Araldite® AV138 (a), Araldite® 2015 (b) and
Sikaforce®_{ 7752 (c). According to Ji et al. [}_{20}_{], }_{G}

IC and *G*IIC are obtained when the

curves reach the steady state value of *G*I/*G*II. The adhesives in study present distinct

ductility, which reflects in the different obtained values of *δ*n/*δ*s corresponding to

*G*IC/*G*IIC. In fact, the adhesives Araldite® 2015 and Sikaforce® 7752 reveal a softening

phase near *G*IC and *G*IIC for the DCB and ENF curves, respectively, due to their

duc-tility. In this work, the DCB specimens of Fig. 6 present the following *G*IC (N/mm):

0.252 (Araldite® AV138), 0.437 (Araldite® 2015) and 3.420 (Sikaforce® 7752). From
the ENF tested specimens presented in Fig. 6, the following *G*IIC values were obtained

(N/mm): 0.479 (Araldite®_{ AV138), 3.444 (Araldite}®_{ 2015) and 5.790 (Sikaforce}®_{ 7752). }

As a result from this work, Table 2 presents the set of *G*IC and *G*IIC values obtained for

each specimen by the *J*-integral technique, with the average and standard deviation
values for each condition. A comparison is also made with previous results obtained

0.0 0.1 0.2 0.3 0.4 0.5 0.6

0 0.025 0.05 0.075 0.1
*G*I

or

*G*II

[N/

mm]

δnor δs[mm]

Tensile curve (DCB) Shear curve (ENF)

0 1 2 3 4

0 0.1 0.2 0.3 0.4 0.5 0.6
*G*I

or

*G*II

[N/

mm]

δnor δs[mm]

Tensile curve (DCB) Shear curve (ENF)

0 2 4 6 8

0 0.2 0.4 0.6 0.8 1
*G*I

or

*G*II

[N/m

m]

δnor δs[mm]

Tensile curve (DCB) Shear curve (ENF)

**a** **b**

**c**

**Fig. 6** Representative *G*_{I}–δ_{n} and G_{II}–δ_{s} curves for the adhesives Araldite® AV138 (**a**), Araldite® 2015 (**b**) and
Sikaforce® 7752 (**c**): raw curve and polynomial approximations

**Table 2 Values of ****G**_{IC} and **G**_{IIC} (N/mm) for the three adhesives

**Adhesive** **Araldite**®_{ AV138}** _{Araldite}**®

_{ 2015}**®**

_{Sikaforce}

_{ 7752}**Specimen** **G****IC** **G****IIC** **G****IC** **G****IIC** **G****IC** **G****IIC**

1 0.224 0.552 0.437 3.444 3.420 –

2 0.252 0.732 0.434 – 3.903 5.067

3 0.231 0.676 0.494 2.873 3.842 6.050

4 0.329 – 0.456 3.298 4.183 5.360

5 0.237 0.566 0.665 3.123 – 6.070

6 0.197 0.533 0.712 3.140 3.502 5.173

7 0.523 3.080 – 5.790

8 0.479 2.901 – 6.160

Average J-int 0.245 ± 0.045 0.580 ± 0.090 0.533 ± 0.123 3.123 ± 0.203 3.770 ± 0.278 5.667 ± 0.459 Average CBBM [18,

by the compliance-based beam method (CBBM) [18, 31, 36]. Some of the tested
spec-imens were not considered for analysis, due to significant deviations from the average
behaviour, or due to difficulties in the CZM law polynomial fitting procedure
dur-ing the application of the direct method. To build the average tensile and shear CZM
laws for further strength prediction of the scarf joints, the average *G*IC and *G*IIC values

referred in Table 2 were considered. However, for the CZM laws, *t*n0 and *t*s0 are also

required. The average values of *t*n0 and *t*s0 were used for this purpose, obtained from the

differentiation procedure applied to *G*I–*δ*n and *G*II–*δ*s curves from the DCB and ENF

tests, respectively, giving the following values (MPa): *t*n0= 37.4 and *t*s0= 16.8 (Araldite®

AV138), *t*n0= 32.9 and *t*s0= 14.8 (Araldite® 2015) and *t*n0= 22.0 and *t*s0= 11.7 (Sikaforce®

7752). By comparing the cohesive parameters, (*t*n0, *t*s0, *G*IC and *G*IIC) and the values

pre-sented in Table 1 for the different adhesives, some deviations can be found. These
differences regard the equivalency between *t*n0 and the tensile strength (*σ*f), and also *t*s0

and the shear strength (*τ*f). However, the obtained *t*n0 and *t*s0 values cannot be directly

compared with the properties *σ*f and *τ*f, since they take into account the constraint

effects caused by the adherends. On the other hand, *G*IC and *G*IIC depend on *t*A and

*t*P of the test specimens which are being used for characterization [37]. Thus, in this

work, the DCB, ENF and scarf geometries were defined to match as best as
possi-ble, regarding *t*A and *t*P. According to Ji et al. [20], although the cohesive parameters

obtained by the direct method do not have a clear physical significance, they are able
to accurately reproduce the materials’ behaviour into a macro scale view point, which
is accurate. Figure 7 represents the CZM laws in tension (*t*n–*δ*n) and shear (*t*s–*δ*s)

corresponding to the specimens of Fig. 6. It can be seen that the tensile and shear behaviour of Araldite® AV138 can be more accurately modelled with a triangular approximation, mainly due to its brittleness. On the other hand, the tensile and shear

0 10 20 30 40 50

0 0.05 0.1 0.15 0.2
*t*n

or

*t*s

[MPa

]

δnor δs[mm]

Tensile law Shear law Simplified CZM laws

0 10 20 30 40

0 0.1 0.2 0.3 0.4 0.5
*t*n

or

*t*s

[MPa

]

δnor δs[mm]

Tensile law Shear law Simplified CZM laws

0 10 20 30

0 0.2 0.4 0.6 0.8

*t*n

or

*t*s

[MPa

]

δnor δs[mm]

Tensile law Shear law Simplified CZM laws

**a** **b**

**c**

laws of Araldite® 2015 and Sikaforce® 7752 are best adjusted by trapezoidal CZM laws, due to the allowable plasticization of the referred adhesives before failure.

**Stress analysis**

A numerical stress analysis was initially carried out to study *σ* and *τ* stresses developing
at the middle of the scarf adhesive layer, during elastic loading, as a function of the
nor-malized scarf length *x*/*L*S (0 ≤*x*≤*L*S), in which *x* is the coordinate tangential to the

adhe-sive layer and *L*S the scarf length. Both *σ* and *τ* stresses were subjected to a normalization

procedure, by dividing them by the average shear stress in the adhesive layer (*τ*avg) for

each *α*. In this work, only the stress distributions for the joints bonded with the Araldite®
2015 are shown. However, these stresses are also representative of the other two
adhe-sives’ behaviour (although there are small differences in the peak stresses because of the
differences in *E*; see Table 1). In general, it is known that the use of smaller values of *α*

leads to higher *L*S and, thus, to higher joint strengths. However, it also provides longer

machined lengths and required volume of adhesive [38].

Figure 8 shows *σ* (a) and *τ* (b) stress distributions for the scarf joints bonded with the
Araldite® 2015, as a function of *α*. It was found that *σ* stresses are much smaller in
mag-nitude than *τ* stresses for the smaller values of *α*, and that these progressively approach

*τ* stresses for *α*= 45°, at which angle both stress components have a similar significance
[39, 40]. This conclusion agrees with the theoretical analyses of references [41, 42]. The
peak *σ* stresses found for the joints with smaller *α* gradually reduce by increasing this
parameter. On the other hand, *τ* stresses keep an identical behaviour along the bond
length, although peak *τ* stresses also tend to become more flat with the increase of *α*

[43]. Actually, considering the scarf joint with *α*= 45°, *τ* stresses are practically constant.
These results seem to indicate that smaller *α* have an improved behaviour because of the
reduction of normalized *σ* stresses, although minor *τ* stress gradients appear for small

*α*. Added to this, smaller *α* also correspond to higher *L*S, which should lead to larger *P*m.

**Damage variable analysis**

This Section addresses a study of the damage variable of the CZM elements (SDEG
vari-able in Abaqus®) across the adhesive layer, i.e. for 0 ≤*x*/*L*S≤ 1, to fully characterize the

failure process of the scarf joints bonded with the three adhesives. The SDEG variable spans between 0 (corresponding to the elastic part of the CZM law) and 1 (or 100%,

0 0.2 0.4 0.6 0.8 1 1.2 1.4 1.6

0 0.2 0.4 0.6 0.8 1

σ

/

τavg

*x*/*L*S

3.43º 10º 15º 20º 30º 45º

0 0.2 0.4 0.6 0.8 1 1.2 1.4 1.6

0 0.2 0.4 0.6 0.8 1

τ

/

τavg

*x*/*L*S

3.43º 10º 15º 20º 30º 45º

**a** **b**

relating to failure of the CZM element). Initially, the SDEG plots of the three adhesives
as a function of *x*/*L*S are presented for the instant of *P*m (Fig. 9). The curves are cropped

at SDEG = 0.3 to improve their visualization.

Notwithstanding the adhesive type, the highest incidence of damage in this type of joint occurs at the adhesive layer’s ends, consistently to the stress distributions presented

in “Introduction” section. Oppositely, at the intermediate zone of the bond, SDEG is

typically zero. Between adhesives, it was found that the stiffness and brittleness of the
Araldite® AV138 makes it very sensible to the peak stresses that take place near *x*/*L*S= 0

and 1 (Fig. 8 shows this effect, although for a different adhesive), such that the span
of damage, i.e., length of *x*/*L*S between SDEG = 0 and 1, is very short. The total length

under damage ranges between 11.1% (*α*= 3.43°) and 55.0% (*α*= 45°) of *L*S, reinforcing

the lack of plasticization ability of this adhesive. The shift in the adhesives’ properties,
particularly the increasing elastic compliance and ductility, enables damage to spread
more evenly and to reduce the gradients along the bond length. Actually, on one hand,
the higher compliance of the Araldite® 2015 and Sikaforce® 7752 reduces *σ* and *τ* peak
stresses which, alone, helps in spreading damage more evenly. On the other hand, the
higher ductility of these two adhesives, compared to the Araldite® AV138, enables the
damaged regions to keep working while the inner regions of the bond are put under
loads as well. As a result, the damage lengths for these adhesives range between 65.0%
(*α*= 45°) and 87.2% (*α*= 3.43°) for the Araldite® 2015 and 15.0% (*α*= 45°) and 78.6%
(*α*= 3.43°) for the Sikaforce® 7752. Between adhesives, the increased compliance of the
Sikaforce® 7752 is responsible for the more uniform span of damage at *P*m, which ranges

between 0 and ≈ 12.5% compared to 0–100% for the Araldite® AV138 and 0–43.8% for

the Araldite® 2015 (maximum values, obtained for specific *α*). Comparing the SDEG
curves between the different *α*, the Araldite® AV138 shows a different behaviour to the
other adhesives, in the sense that smaller *α* results in more concentrated damage and

0 0.1 0.2 0.3

0 0.2 0.4 0.6 0.8 1

SD

EG

*x/LS*

3.43º 10º 15º 20º 30º 45º

0 0.1 0.2 0.3

0 0.2 0.4 0.6 0.8 1

SDEG

*x*/*L*S

3.43º 10º 15º 20º 30º 45º

0 0.1 0.2 0.3

0 0.2 0.4 0.6 0.8 1

SDEG

*x*/*L*S

3.43º 10º 15º 20º 30º 45º

**a** **b**

**c**

higher SDEG gradients. This is because of its brittleness, which clearly cannot
accom-modate the higher *σ* and *τ* peak stresses at the overlap ends (this effect can be identified
in Fig. 8, despite this figure relates to the Araldite® 2015). Since *σ* and *τ* stresses slowly
become more flat with increasing *α*, the damage also increases towards the central
region of the bond. The ductile adhesives are not affected by these peak stresses, since
the damage span across the bond does not vary much with *α*. Nonetheless, SDEG attains
higher percentile values at *P*m for smaller *α* also due to the aforementioned differences in

*σ* and *τ* peak stresses.

**Discussion on the joint strength**

All failures were cohesive in the adhesive layer. Figure 10 shows, as an example, the
fracture surfaces for the scarf joints bonded with the Sikaforce® 7752 and *α*= 3.43°.
Fig-ure 11 compares the experimental *P*m values of the scarf joints bonded with the three

adhesives as a function of *α*. The obtained results showed that the mechanical behaviour

**Fig. 10** Fracture surfaces for the scarf joints bonded with the Sikaforce® 7752 and α = 3.43°

0 5 10 15 20 25 30 35

0 10 20 30 40 50

*P*m

[k

N]

α[º]

AV138 2015 7752

of the scarf joints is highly dependent on the type of adhesive and value of *α*. Actually,
a more stiff and brittle adhesive leads to higher peak stresses and instability in damage
propagation, while a less stiff and ductile adhesive presents more uniform stress
distri-butions and more stable damage growth during loading. This also translated into a
dif-ferent damage behaviour, with the SDEG variable showing abrupt variations along *x*/*L*S

for the Araldite® AV138, thus concentrating along a smaller bond length. Oppositely,
for the other two adhesives, due to their higher compliance and ability to undergo the
plastic regime of the adhesive, the damage spreads more evenly and a larger portion of
the adhesive layer is contributing to the load transfer. A difference in *P*m is also evident

with the decrease of *α*. Actually, smaller *α* promote an increase of stress concentrations
[44] and increasing SDEG gradients along the bond length, which could be
responsi-ble for a *P*m reduction. However, smaller values of *α* have the advantage of presenting

an increasingly larger bond length and area, which cancels the peak stresses effect and
results in much higher *P*m values. The *P*m evolution with *α* is typically exponential, which

agrees with previous results [6]. In fact, a significant increase in strength was found
for *α* smaller than 20°, while for bigger *α* the differences are minimal. In the
particu-lar case of the Araldite®_{ AV138, there is a 67% }_{P}

m increase from *α*= 45° to 20°, and a

445% *P*m improvement between *α*= 20° to 3.43°. By the same respective order, for the

Araldite® 2015, these percentile *P*m differences are 95% and 492% and, for the Sikaforce

7752, these are 99% and 439%. By comparing the three adhesives, the Araldite® AV138
gives the best results for all *α*, although it is the most brittle. Actually, the *P*m variation

over the Araldite®_{ 2015 ranges from 37.4% (}_{α}_{=}_{ 10°) to 78.1% (}_{α}_{=}_{ 45°). Compared to the }

Sikaforce® 7752, these differences are 120.6% (*α*= 10°) and 182.8% (*α*= 30°). This
behav-iour is somehow different to the typical behavbehav-iour of lap-joints, in which strong yet
brit-tle adhesives are clearly outperformed by less strong but more ductile adhesive [45].
However, in these cases, large peak stresses exist at the overlap edges, which make joints
with brittle adhesive to fail prematurely, without any ability to undergo plastic behaviour
and stress redistribution. On the other hand, joints with ductile adhesives manage to
undergo plastic deformations in the adhesive layer after the limiting stresses are attained,
which increases the average stress at failure in the bondline and, correspondingly, *P*m is

also higher [46]. The contrasting behaviour observed for the scarf joints tested in this work is mainly due to the much smaller stress gradients than in lap joints (Fig. 8), leading to best results with a stronger but brittle adhesive because, under these conditions, the average stress at failure is higher. These findings agree with previous results [47], relating to hybrid scarf joints between aluminium and composites. On the other hand, the adhe-sives’ ductility is not as important as in lap joints.

**Evaluation of the different CZM law shapes**

Figure 12a–c present the comparison between the experimental *P*m and the respective

for all geometric conditions and adhesives, emphasizing that the strength
predic-tion of adhesive joints by CZM modelling using a direct method for the cohesive laws’
estimation is accurate. Moreover, this analysis showed which CZM law shape is best
suited for each type of adhesive, although the differences between CZM shapes is very
small. The analysis showed that this was due to a typically uniform stress state. It was
also found that, as the adhesives’ ductility increases, the percentile deviation between
CZM law shapes becomes smaller. The maximum differences between the mixed-mode
and independent-mode formulations were 1.66% for the Araldite® AV138, 0.74% for
the Araldite® 2015 and 0.68% for the Sikaforce® 7752. For all adhesives, the percentile
reduction between the mixed-mode and independent-mode models also reduces with
increasing *α*. On the other hand, previous studies revealed that, in other geometries,
much higher differences can be found [24]. However, for the particular set of conditions
tested in this work, the CZM law shape is irrelevant. Nonetheless, for each adhesive, a
CZM formulation exists that performs slightly better than the other. The match between
the independent-mode models and the mixed-mode model also depends on the
adhe-sive type. For the Araldite® AV138, the triangular independent-mode model approaches
most to the mixed-mode model. The deviations between these two formulations range
from 0.1% (*α*= 45°) to 0.5% (*α*= 3.43°). For the Araldite® 2015, the trapezoidal
inde-pendent-mode model gives the best match to mixed-mode model, with deviations from
0.2% for *α*= 45° to 0.5% for *α*= 3.43°. The differences are minimal between

independent-mode independent-models when using the Sikaforce® 7752. Nonetheless, the exponential model gives
slightly closer values to the mixed-mode model. The obtained differences were between
0.2% for *α*= 45° and 0.7% for *α*= 3.43°.

Figure 13 represents the evolution of percentile difference between *P*m for each

inde-pendent model and the mixed-mode triangular model (Δ) with *α*, for the three tested

0 5 10 15 20 25 30 35

0 10 20 30 40 50

*P*m

[k

N]

α[º]

Experimental Mixed Tri Trap Exp

0 4 8 12 16 20 24 28

0 10 20 30 40 50

*P*m

[k

N]

α[º]

Experimental Mixed Tri Trap Exp

0 2 4 6 8 10 12 14 16

0 10 20 30 40 50

*P*m

[k

N]

α[º]

Experimental Mixed Tri Trap Exp

**a** **b**

**c**

adhesives. An overlook of the results shows that, in all cases, Δ acquires negligible
val-ues. This reinforces that, for the particular tested conditions (practically uniform stress
distributions; Fig. 8), the influence of coupling the loading modes in the CZM laws has
a marginal effect. The largest absolute difference between any independent-mode law
and the mixed-mode triangular law were 1.66% for the Araldite® AV138 (exponential
model), 0.74% for the Araldite®_{ 2015 (exponential model) and 0.68% for the Sikaforce}®

7752 (triangular model), in all cases for the smallest *α*. A marked tendency was found
to reduce Δ with the increase of the adhesives’ ductility, although this occurs with a less
extent for the Sikaforce® 7752. On the other hand, this also reflects on corresponding
smaller deviations between the different independent-mode models. Inclusively, for the
scarf joints bonded with the Sikaforce®_{ 7752, the results are virtually identical. In more }

detail, the largest absolute deviations between the trapezoidal or exponential independ-ent-mode laws over the triangular independindepend-ent-mode law were 1.22% for the Araldite® AV138, 0.14% for the Araldite® 2015 and 0.02% for the Sikaforce® 7752, which clearly shows this trend. This reinforces the conclusions of Fig. 12, which showed that, under the testing conditions, the influence of both law shape and mode coupling is negligible. As a result, for this type of joint, mode uncoupling and any law type can be used with confidence in the strength prediction. This is also valid for the simulation of composite delaminations [48]. It should however be noted that, in joint configurations that induce higher stress gradients along the overlap, the differences due to using a less conveni-ent CZM law shape can increase. Campilho et al. [27] attained differences in order of magnitude of 10% by simulating single-lap joints bonded with the Araldite® 2015 with a triangular CZM.

-2 -1.5 -1 -0.5 0 0.5 1

0 10 20 30 40 50

∆

[%

]

α[º] Tri Trap Exp

-2 -1.5 -1 -0.5 0 0.5 1

0 10 20 30 40 50

∆

[%

]

α[º] Tri Trap Exp

-1 -0.75 -0.5 -0.25 0

0 10 20 30 40 50

∆

[%

]

α[º] Tri Trap Exp

**a** **b**

**c**

**Conclusions**

The main purpose of this work was the evaluation of different CZM formulations to
predict the strength of adhesively-bonded scarf joints, considering the tensile and
shear pure-mode laws were estimated by a direct method. Three adhesives were
evaluated, whose behaviour ranged from strong and brittle to less strong and ductile.
The results showed that the mechanical behaviour of the scarf joints is dependent on
the type of adhesive and value of *α*. A more stiff and brittle adhesive leads to slightly
higher peak stresses, while a more flexible and ductile adhesive gives more uniform
stress distributions. Nonetheless, comparing with other joint configurations such as
single-lap and double-lap, the stress distributions are much improved. Peak *τ* stresses
along the bondline increase with the reduction of *α*, which negatively affects the joint
strength, but the reduction of this parameter also increases exponentially *L*S, whose

effect is much more preponderant and leads to a *P*m improvement. The damage plots

at *P*m reflected the result of the elastic stress distributions, with maximum damage

at the adhesive ends. The damage span was smallest for the Araldite® AV138, due to
the combined effect of the highest peak stresses and reduced *G*IC and *G*IIC, while the

other adhesives showed an improved behaviour by enabling a wide damage spread at

*P*m. Despite these facts, the experimental *P*m results showed that the Araldite® AV138

achieves the highest *P*m for all *α* between adhesives because, under the conditions

of small stress gradients, the strengths of the adhesive are prevalent over the energy parameters. The numerical strength predictions were accurate in comparison with the experimental data, for all CZM law shapes and coupling modes. For the particu-lar geometry tested in this work, the differences between CZM shapes were minimal. Thus, no significant errors are made in the choice of a less adequate law. However, it should be noted that this only occurs due to the particular load transfer characteris-tics of scarf joints. For other geometries, namely with higher stress gradients along the adhesive, non-negligible differences can be found between law shapes.

**Abbreviations**

2D: two-dimensional; a: crack length; a0: initial crack length; B: width; CZM: cohesive zone models; DCB:
double-Cantile-ver Beam; dn: damage variable in tension; ds: damage variable in shear; E: Young’s modulus; ENF: End-Notched Flexure; Ex:
Young’s modulus of the adherends; FEM: finite element method; G: shear modulus; GI: tensile strain energy release rate;
*G*IC: critical tensile strain energy release rate; GII: shear strain energy release rate; GIIC: critical shear strain energy release
rate; L: length (for the DCB specimen) or mid-span (for the ENF test); LO: overlap length; LS: scarf length; LT: length; MMB:
mixed-mode bending; P: load; Pm: maximum load; Pu: load per unit width applied at the specimen ends; SDEG: damage
variable; tA: adhesive thickness; tn: cohesive stress in tension; tn0: cohesive strength in tension; tnund: current value of tn
with-out stiffness loss; tP: adherends’ thickness; ts: cohesive stress in shear; ts0: cohesive strength in shear; tsund: current value of ts
without stiffness loss; x: coordinate tangential to the adhesive layer; XFEM: extended finite element method; Δ: percentile
difference between Pm for each independent model and the mixed-mode triangular model; α: scarf angle; αexp:
param-eter to specify the softening evolution; δ: displacement; δn: relative displacement in tension; δn0: relative displacement at
*t*n0; δnf: tensile relative displacement at failure; δns: tensile stress softening onset displacement of the trapezoidal CZM law;
*δ*s: relative displacement in shear; δs0: relative displacement at ts0; δsf: shear relative displacement at failure; δss: shear stress
softening onset displacement of the trapezoidal CZM law; ε: strain; εn: tensile strain; εs: shear strain; θo: relative rotation
of the adherends at the crack tip; θp: relative rotation of the adherends measured at the loading line; σ: peel stresses; σ:
stress; σf: tensile strength; τ: shear stresses; τavg: average shear stress in the adhesive layer; τf: shear strength.

**Authors’ contributions**

DFOS performed the experimental tests and respective data analysis, and he also performed the numerical analysis. RDSGC and UTFC developed the numerical technique and participated the paper writing. FJGdaS participated in the paper writing. All authors read and approved the final manuscript.

**Author details**

**Acknowledgements**

The authors would like to thank Sika® Portugal for supplying the adhesive.

**Competing interests**

The authors declare that they have no competing interests.

**Availability of data and materials**

The datasets used and/or analysed during the current study are available from the corresponding author on reasonable request.

**Funding**

No funding was received.

**Publisher’s Note**

Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.

Received: 24 October 2018 Accepted: 13 December 2018

**References**

1. Petrie EM. Handbook of adhesives and sealants. New York: McGraw-Hill; 2000.

2. Li J, Yan Y, Zhang T, Liang Z. Experimental study of adhesively bonded CFRP joints subjected to tensile loads. In J Adhes Adhes. 2015;57:95–104. https ://doi.org/10.1016/j.ijadh adh.2014.11.001.

3. Grant LDR, Adams RD, da Silva LFM. Experimental and numerical analysis of single-lap joints for the automotive industry. Int J Adhes Adhes. 2009;29(4):405–13. https ://doi.org/10.1016/j.ijadh adh.2008.09.001.

4. Llopart PL, Tserpes KI, Labeas GN. Experimental and numerical investigation of the influence of imperfect bonding on the strength of NCF double-lap shear joints. Compos Struct. 2010;92(7):1673–82. https ://doi.org/10.1016/j.comps truct .2009.12.001.

5. Gleich DM, Van Tooren MJL, De Haan PAJ. Shear and peel stress analysis of an adhesively bonded scarf joint. J Adhes Sci Technol. 2000;14(6):879–93. https ://doi.org/10.1163/15685 61007 42942 .

6. Moreira RDF, Campilho RDSG. Strength improvement of adhesively-bonded scarf repairs in aluminium structures with external reinforcements. Eng Struct. 2015;101:99–110. https ://doi.org/10.1016/j.engst ruct.2015.07.001. 7. Moreira RDF, Campilho RDSG. Parametric study of the reinforcement geometry on tensile loaded scarf adhesive

repairs. J Adhes. 2016;92(7–9):586–609. https ://doi.org/10.1080/00218 464.2015.10956 39.

8. Volkersen O. Die nietkraftoerteilung in zubeanspruchten nietverbindungen konstanten loschonquerschnitten. Luftfahrtforschung. 1938;15:41–7.

9. Goland M, Reissner E. The stresses in cemented joints. J Appl Mech. 1944;66:A17–27.

10. Penado FE. A simplified method for the geometrically nonlinear analysis of the single lap joint. J Thermoplast Com-pos. 1998;11(3):272–87. https ://doi.org/10.1177/08927 05798 01100 306.

11. Li WD, Ma M, Han X, Tang LP, Zhao JN, Gao EP. Strength prediction of adhesively bonded single lap joints under salt spray environment using a cohesive zone model. J Adhes. 2016;92(11):916–37. https ://doi.org/10.1080/00218 464.2015.10581 64.

12. Kafkalidis MS, Thouless MD. The effects of geometry and material properties on the fracture of single lap-shear joints. Int J Solids Struct. 2002;39(17):4367–83. https ://doi.org/10.1016/S0020 -7683(02)00344 -X.

13. Mubashar A, Ashcroft IA, Crocombe AD. Modelling damage and failure in adhesive joints using a combined XFEM-cohesive element methodology. J Adhes. 2014;90(8):682–97. https ://doi.org/10.1080/00218 464.2013.82658 0. 14. Pascoe JA, Alderliesten RC, Benedictus R. Methods for the prediction of fatigue delamination growth in composites

and adhesive bonds—a critical review. Eng Fract Mech. 2013;112–113:72–96. https ://doi.org/10.1016/j.engfr acmec h.2013.10.003.

15. Anyfantis KN, Tsouvalis NG. A novel traction–separation law for the prediction of the mixed mode response of ductile adhesive joints. Int J Solids Struct. 2012;49(1):213–26. https ://doi.org/10.1016/j.ijsol str.2011.10.001. 16. Turon A, Dávila CG, Camanho PP, Costa J. An engineering solution for mesh size effects in the simulation of

delami-nation using cohesive zone models. Eng Fract Mech. 2007;74(10):1665–82. https ://doi.org/10.1016/j.engfr acmec h.2006.08.025.

17. Rocha RJB, Campilho RDSG. Evaluation of different modelling conditions in the cohesive zone analysis of single-lap bonded joints. J Adhes. 2018;94(7):562–82. https ://doi.org/10.1080/00218 464.2017.13071 07.

18. Azevedo JCS, Campilho RDSG, da Silva FJG, Faneco TMS, Lopes RM. Cohesive law estimation of adhesive joints in mode II condition. Theor Appl Fract Mech. 2015;80:143–54.

19. Andersson T, Stigh U. The stress–elongation relation for an adhesive layer loaded in peel using equilibrium of ener-getic forces. Int J Solids Struct. 2004;41(2):413–34. https ://doi.org/10.1016/j.ijsol str.2003.09.039.

20. Ji G, Ouyang Z, Li G, Ibekwe S, Pang S-S. Effects of adhesive thickness on global and local Mode-I interfacial fracture of bonded joints. Int J Solids Struct. 2010;47(18–19):2445–58. https ://doi.org/10.1016/j.ijsol str.2010.05.006. 21. Leffler K, Alfredsson KS, Stigh U. Shear behaviour of adhesive layers. Int J Solids Struct. 2007;44(2):530–45. https ://doi.

org/10.1016/j.ijsol str.2006.04.036.

22. Jumel J, Ben Salem N, Budzik MK, Shanahan MER. Measurement of interface cohesive stresses and strains evolutions with combined mixed mode crack propagation test and backface strain monitoring measurements. Int J Solids Struct. 2015;52:33–44. https ://doi.org/10.1016/j.ijsol str.2014.09.004.

24. Carvalho UTF, Campilho RDSG. Validation of pure tensile and shear cohesive laws obtained by the direct method with single-lap joints. Int J Adhes Adhes. 2017;77(Supplement C):41–50. https ://doi.org/10.1016/j.ijadh adh.2017.04.002.

25. Campilho RDSG, Banea MD, Pinto AMG, da Silva LFM, de Jesus AMP. Strength prediction of single- and double-lap joints by standard and extended finite element modelling. Int J Adhes Adhes. 2011;31(5):363–72. https ://doi. org/10.1016/j.ijadh adh.2010.09.008.

26. Neto JABP, Campilho RDSG, da Silva LFM. Parametric study of adhesive joints with composites. Int J Adhes Adhes. 2012;37:96–101. https ://doi.org/10.1016/j.ijadh adh.2012.01.019.

27. Campilho RDSG, Banea MD, Neto JABP, da Silva LFM. Modelling adhesive joints with cohesive zone models: effect of the cohesive law shape of the adhesive layer. Int J Adhes Adhes. 2013;44:48–56. https ://doi.org/10.1016/j.ijadh adh.2013.02.006.

28. Faneco T, Campilho R, Silva F, Lopes R. Strength and fracture characterization of a novel polyurethane adhesive for the automotive industry. J Test Eval. 2017;45(2):398–407. https ://doi.org/10.1520/JTE20 15033 5.

29. Wang H, Hao X, Yan K, Zhou H, Hua L. Ultrasonic vibration-strengthened adhesive bonding of CFRP-to-aluminum joints. J Mater Process Technol. 2018;257:213–26. https ://doi.org/10.1016/j.jmatp rotec .2018.03.003.

30. Rice JR. A path independent integral and the approximate analysis of strain concentration by notches and cracks. J Appl Mech. 1968;35(2):379–86. https ://doi.org/10.1115/1.36012 06.

31. Constante CJ, Campilho RDSG, Moura DC. Tensile fracture characterization of adhesive joints by standard and opti-cal techniques. Eng Fract Mech. 2015;136:292–304. https ://doi.org/10.1016/j.engfr acmec h.2015.02.010.

32. Leitão ACC, Campilho RDSG, Moura DC. Shear characterization of adhesive layers by advanced optical techniques. Exp Mech. 2016;56:493–506. https ://doi.org/10.1007/s1134 0-015-0111-4.

33. Abaqus®. Documentation of the software Abaqus®. Vélizy-Villacoublay: Dassault Systèmes; 2013.

34. Tsai MY, Morton J. An investigation into the stresses in double-lap adhesive joints with laminated composite adher-ends. Int J Solids Struct. 2010;47(24):3317–25. https ://doi.org/10.1016/j.ijsol str.2010.08.011.

35. Liao L, Huang C, Sawa T. Effect of adhesive thickness, adhesive type and scarf angle on the mechanical properties of scarf adhesive joints. Int J Solids Struct. 2013;50(25):4333–40. https ://doi.org/10.1016/j.ijsol str.2013.09.005. 36. Campilho RDSG, Moura DC, Banea MD, da Silva LFM. Adhesive thickness effects of a ductile adhesive by optical

measurement techniques. Int J Adhes Adhes. 2015;57:125–32. https ://doi.org/10.1016/j.ijadh adh.2014.12.004. 37. Lee D-B, Ikeda T, Miyazaki N, Choi N-S. Effect of bond thickness on the fracture toughness of adhesive joints. J Eng

Mater Tech. 2004;126(1):14–8. https ://doi.org/10.1115/1.16314 33.

38. Afendi M, Teramoto T, Bakri HB. Strength prediction of epoxy adhesively bonded scarf joints of dissimilar adherends. Int J Adhes Adhes. 2011;31(6):402–11. https ://doi.org/10.1016/j.ijadh adh.2011.03.001.

39. Imanaka M, Fujinami A, Suzuki Y. Fracture and yield behavior of adhesively bonded joints under triaxial stress condi-tions. J Mater Sci. 2000;35(10):2481–91. https ://doi.org/10.1023/A:10047 69719 895.

40. Imanaka M, Suzuki Y. Yield behavior of rubber-modified epoxy adhesives under multiaxial stress conditions. J Adhes Sci Technol. 2002;16(12):1687–700. https ://doi.org/10.1163/15685 61026 02552 88.

41. Objois A, Fargette B, Gilibert Y. The influence of the bevel angle on the micro-mechanical behaviour of bonded scarf joints. J Adhes Sci Technol. 2000;14(8):1057–70. https ://doi.org/10.1163/15685 61007 43077 .

42. Objois A, Assih J, Troalen JP. Theoretical method to predict the first microcracks in a scarf joint. J Adhesion. 2005;81(9):893–909. https ://doi.org/10.1080/00218 46050 02228 19.

43. Odi RA, Friend CM. An improved 2D model for bonded composite joints. Int J Adhes Adhes. 2004;24(5):389–405. https ://doi.org/10.1016/j.ijadh adh.2001.06.001.

44. Wang CH, Gunnion AJ. On the design methodology of scarf repairs to composite laminates. Compos Sci Technol. 2008;68(1):35–46. https ://doi.org/10.1016/j.comps citec h.2007.05.045.

45. Adams RD, Mallick V. The effect of temperature on the strength of adhesively-bonded composite-aluminium joints. J Adhes. 1993;43(1–2):17–33. https ://doi.org/10.1080/00218 46930 80265 85.

46. Davis M, Bond D. Principles and practices of adhesive bonded structural joints and repairs. Int J Adhes Adhes. 1999;19(2–3):91–105. https ://doi.org/10.1016/S0143 -7496(98)00026 -8.

47. Alves DL, Campilho RDSG, Moreira RDF, Silva FJG, da Silva LFM. Experimental and numerical analysis of hybrid adhesively-bonded scarf joints. Int J Adhes Adhes. 2018;83:87–95. https ://doi.org/10.1016/j.ijadh adh.2018.05.011. 48. Yang Q, Cox B. Cohesive models for damage evolution in laminated composites. Int J Fract. 2005;133(2):107–37.